International Temper Designation Systems for Wrought Aluminum
Reprinted with permission, ©2009 Light Metal Age
International Temper Designation Systems for
Wrought Aluminum Alloys:
Part I – Strain Hardenable (H Temper) Aluminum Alloys
By Joseph C. Benedyk, Editor
s the need arose in the aluminum industry to
describe standard temper treatments and establish uniform temper designations, The Aluminum Association has served as the main body
registering aluminum alloys and temper designations
in its ANSI H35.1 standard. This standard dates back to
1957 (American Standard H35.1-1957), when it consisted
only of the designation system for wrought aluminum alloys that was originally developed by The Aluminum Association. The ANSI H35.1 standard was reissued in 1962
to add the temper designation system in effect in the U.S.
since 1948. It has been revised many times over the years
and since 1971 has been published by The Aluminum
Association, Inc., the Secretariat for the Accredited Standards Committee (ASC) H35.
The Aluminum Association is the registrar under ANSI
H35.1/H35.1(M) with regard to the designation and
composition of wrought aluminum alloys and tempers
registered in the U.S. and also the registrar under an international accord on the composition and designation
of wrought aluminum alloys. The international alloy designations and chemical composition for wrought aluminum and wrought aluminum alloys are registered in the
latest Teal Sheets 2009 published by The Aluminum Association in February 2009 as a revision to the April 2006
document; the publication of Teal Sheets 2009 is available
as a free downloadable pdf from The Aluminum Association website: www.aluminum.org/tealsheets, as well as
from the European Aluminium Association website: www.
The latest document on ANSI alloy and temper designation systems for aluminum—ANSI H35.1/H35.1(M)20091—published by The Aluminum Assocation, Inc. is
a revision of ANSI H35.1/H35.1(M)-2006. The edition
combines the U.S. and metric versions of this publication,
as the metric edition (ANSI H35.1M) has not been published as a separate document since 2004.
With regard to tempers of aluminum alloys, ANSI
H35.1/H35.1(M)-2009 varies from the 2006 version in
that new definitions were applied to assigned additional
digits for T7 (overaged) temper variations as well as other
clarifications of temper designations. The ANSI H35.1/
H35.1(M)-2009 document also appears in its entirety in
Aluminum Standards and Data 2009,2 recently published
by The Aluminum Association. As mentioned in Aluminum Standards and Data 2009 and in the preface to the
ANSI H35.1/H35.1(M)-2009 section on temper designations: “Since there is no international accord on designation and registration of tempers for wrought aluminum
alloys and wrought aluminum alloy products, reference
to ANSI H35.1/H35.1(M) may not always reflect actual
properties and characteristics associated with the particular aluminum alloy temper.”
This may be changing, slowly but surely. As late as 2003,
there was no international accord for aluminum and aluminum alloy temper designations or temper registrations
that served as product standards.3 However, the global
restructuring of the aluminum industry has made it imperative that aluminum alloy standards become more
universal in order to assure consistency in the purchase
and use of aluminum products worldwide. In this respect,
the ANSI H35.1/H35.1(M) standard was the basis for ISO
2107, which is an attempt to unify the worldwide aluminum temper designation system. Yet differences in temper designations for wrought aluminum and aluminum
alloys still exist from country to country. Even between
the U.S. and European member countries of CEN (Comité Européen de Normalisation/European Committee
for Standardization), where the EN 515 standard is very
similar to the wrought alloy portion of ANSI H35.1 (M).4
Some differences are noted in the respective temper designations and standards as late as 2008.5
Within the EAA (European Aluminium Association),
the management of the EAA Standards Committee and
all its interactions with European standardization activities relating to aluminum semi-products, castings, and alloys are now coordinated within the Gesamtverband der
Aluminiumindustrie e.V./General Association of the Aluminum Industry (GDA), which took over responsibility
for this field from EAA in 2008.6 Teal Sheets 2009 is also
available as a free download from the GDA website: www.
However, the Aluminum and Aluminum Alloys Technical
Committee of the European Committee for Standardization (CEN/TC 132) is the group focusing on European
standardization for aluminum products, including EN
515 for wrought alloy temper designations.
This article (Part I) attempts to summarize the latest
information on temper designations and definitions established worldwide for wrought aluminum alloys under
the general classification of strain-hardened (H temper).
A subsequent article (Part II) will focus on thermally
treated or heat treatable (T temper) wrought aluminum
alloy tempers. Wrought aluminum alloys in the strain
hardened (H temper) class are generally 1xxx, 3xxx, and
5xxx alloys, while those classified as thermally treated or
heat treatable (T temper) are generally 2xxx, 6xxx, and
7xxx alloys. Finally, Part III will cover temper designations for casting alloys.
In this article, H temper designations in the ANSI
H35.1/H35.1(M)-2009 standard will be reviewed with
respect to changes from ANSI H35.1/H35.1(M)-2006,
differences between the temper designations used in the
U.S. under ANSI H35.1(M) and in Europe in CEN countries under EN 515 (Wrought Products/Temper Designations) will be noted, and some comparisons will be made
with older temper designations used in various countries.
For example, the older and now outdated DIN (Deutches Institut für Normung/German Industry Standard)
and BS (British Standard) designations for aluminum
tempers have been used in technical publications up to
1988 and perhaps later.7 A comparison between the old
and new systems is thus important if previously published
knowledge on aluminum alloys is to be readable by those
unfamiliar with the old system.
Basic Temper Designations of Wrought Aluminum Alloys
The ANSI H35.1/H35.1(M)-2009 temper designation
system for all wrought aluminum alloys follows the alloy
designation with the two separated by a hyphen. The basic temper designations in this system consist of the letters
F, O, H, W, or T indicating the general process of product
LIGHT METAL AGE, OCTOBER 2009
manufacture or heat treatment (Table I). Subdivisions of
the basic tempers are indicated by one or more digits that
follow the letter, e.g., 1100-H14, 3003-O, 3004-H38, 5052H32, 5083-H116, 5456-H321, etc. for strain hardenable
aluminum alloys of the 1xxx, 3xxx, and 5xxx series, and
2024-T62, 6061-T451, 7075-T7351, etc. for heat treatable
aluminum alloys of the 2xxx, 6xxx, and 7xxx series.
designation stands alone.
As is typical of the effect of cold work on metals, the
driving force for recrystallization in annealing is higher
as the degree of cold work (strain-hardening) increases,
thus resulting in a lower recrystallization temperature
for annealing. Also, a high degree of cold work typically
results in a finer recrystallized grain size upon annealing
at recommended temperatures. Normally undesirable,
coarse grains lead to a reduction in strength and ductility
and can occur due to secondary recrystallization upon annealing of strain-hardened aluminum alloys at high temperatures (e.g., >1,000°F). Critical values of cold work of
2-15% in aluminum alloys can foster coarse grain growth
during annealing at recommended temperatures that are
well below 1,000°F. The recrystallization temperature is affected to varying degrees by the alloying elements; in aluminum alloys, alloying elements such as Mn, Cr, and Fe
increase recrystallization temperature. In 5xxx alloys, for
example, Mn levels above 0.6% increase recrystallization
temperature to such an extent that recrystallization may
be retarded during hot rolling, extrusion, or forging.
Table I. Basic temper designations per ANSI H35.1/H35.1(M)-2009
and adopted by the European EN 515 temper designation system.
Temper Designations Systems for
Wrought Strain Hardenable Aluminum Alloys
Wrought aluminum alloys of the 1xxx, 3xxx, and 5xxx
series are hardened by cold working, i.e., they are strain
hardenable and not hardened to any significant degree
by age hardening heat treatments. In sum total, Teal
Sheets 2009 and its June 2009 addendum list 41 1xxx
alloys, 48 3xxx alloys, and 96 5xxx alloys for a total of
185 internationally registered wrought strain hardenable
aluminum alloys. As for all aluminum alloys, the temper
designations for strain hardenable aluminum alloys are
given after the alloy, e.g., 1100-H14, 3003-O, 3004-H38,
5052-H32, 5083-H116, 5456-H321, etc.
Temper designations for wrought strain hardenable
aluminum alloys in the U.S. (ANSI H35.1/H35.1(M)
The ANSI H35.1/
and EN 515
of -F for as
of -F for as fabricated
the past in used
are no countries,
can be easily
be easily compared
the recent with
III. in Table III.
Full Annealing – O Temper
The O temper designation is applied to the fully annealed metallurgical condition that achieves complete
recrystallization of the alloy, yielding the lowest strength,
highest ductility, and the most workable characteristics.
The O temper designation is used for all aluminum alloys, whether or not they are strain-hardenable or heattreatable. Annealing practices (temperature, time, and
heating and cooling rates) vary depending on the type
of aluminum alloy and prior metallurgical condition. For
the strain-hardenable aluminum alloys, the O temper
Table II. ANSI H35.1 temper designation system used presently in the
U.S. and CEN member European countries, as well as ISO 2107, for
strain hardened wrought aluminum and aluminum alloys.
Strain Hardened, Partially Annealed, Stabilized – H Tempers
In the strain hardened (H) tempers, the subsequent
suffix digits indicate the particular treatments, described
in Table II, used to achieve specified properties in given
1xxx, 3xxx, and 5xxx strain hardenable alloy products
based on the respective product standards. The first suffix digit after H (Hx) indicates the type of treatment used
to affect physical or mechanical properties in these alloys:
LIGHT METAL AGE, OCTOBER 2009
Table III. Comparison of temper designations used in the U.S., CEN member European countries, and different or older standards for strain
hardenable wrought aluminum alloys.1,4-7
1 – strain hardened by cold work only, 2 – cold worked
more than desired amount and partially annealed, 3
– cold worked and stabilized, and 4 – cold worked and
partially annealed due to lacquering or paint baking operations.
Cold working of these alloys is most often imparted
by cold rolling, as sheet and plate are the most common
1xxx, 3xxx, and 5xxx alloy products available, although
cold working can also be imparted by drawing, forging,
or other metalworking process. As presented in Table
II, the second suffix digit after H (H--_x) indicates the
degree of residual hardening (H_1 – 1/8 hard to H_9
– extra hard) with tensile property specifications established for each set of digits. H1 (cold worked) tempers
are preferred over H2 (cold worked more than the desired amount and partially annealed) tempers, because
partial annealing requires precise temperature control
to achieve the required mechanical properties, especially
at high levels of cold work. H3 (strain hardened and stabilized) tempers for 5083 involve heating to soften and
stabilize mechanical properties to improve forming.
LIGHT METAL AGE, OCTOBER 2009
Marine Markets – H116 and H321 Tempers
As part of the efforts by the aluminum industry to eliminate potential problems in the selection of aluminum
alloys and tempers for the marine market, The Aluminum Association has modified the definitions of both
the H116 and H321 tempers of 5xxx aluminum alloys
with magnesium contents above 3%.8 Product forms for
5xxx-H116 and 5xxx-H321 are almost exclusively sheet
and plate. Prior to 2004, the H116 temper only required
exfoliation corrosion resistance testing, and the H321
temper required no corrosion testing. Present requirements for 5xxx alloys with magnesium contents above
3%, approved by ASC H35 and published for the first
time in ANSI H35.1/H35.1(M)-2004, maintained in
ANSI H35.1/H35.1(M)-2009, and adopted in ASTM B
928/B 928-2007,9 specify H116 and H321 for continuous
service at temperatures no greater than 150°F in marine
environments, and are as follows:1
•H116 – Applies to products manufactured from alloys
in the 5xxx series, for which the magnesium content is
3% nominal or more. Products are strain hardened at
the last operation to specified stable tensile property
limits and meet specified levels of corrosion resistance
in accelerated type corrosion tests. They are suitable for
continuous service at temperature no greater than 150°F
(66°C). Corrosion tests include intergranular and exfoliation.
•H321 – Applies to products from alloys in the 5xxx
series, for which the magnesium content is 3% nominal
or more. Products are thermally stabilized after the last
operation to specified stable tensile property limits and
meet specified levels of corrosion resistance in accelerated corrosion tests. Corrosion tests include intergranular and exfoliation.
The marine service alloys and tempers include 5059H116, 5059-H321, 5083-H116, 5083-H321, 5086-H116,
for which and
tested to pass
9 as defined in ASTM B
tests as defined in ASTM B 928.
Intergranular and Exfoliation Corrosion Tests
for H116 and H321 Tempers
The resistance to intergranular corrosion of individual lots of 5xxx-H116 and/or –H321 products is determined by the ASTM G 67 test or nitric acid mass loss
test (NAMLT) and microscopic examination to assure a
microstructure that is predominantly free of a continuous grain boundary network of aluminum-magnesium
precipitate, often termed beta-phase. The beta-phase is
highly anodic relative to the 5xxx alloy matrix. In the
conduct of the NAMLT, mass loss after immersion in a
concentrated nitric acid solution (70-72 wt%) at 86°F for
24 hours should be no greater than 15 mg/in2 for absolute pass acceptance, while samples with a mass loss of
15.5-25 mg/in2 need to be metallographically examined
and compared with acceptable reference photomicrographs to assure pass acceptance.
Exfoliation corrosion occurs in products with a structure consisting of elongated and oriented grains and is
caused by corrosion along stratified distributions of an
anodic phase, i.e., the beta-phase in 5xxx alloys with magnesium contents greater than 3%. In the conduct of the
ASTM G 66 test or ammonium salt solution exfoliation
test (ASSET), samples immersed for 24 hours in a solution containing ammonium chloride, nitrate, tartrate,
and hydrogen peroxide at 150°F are subjected to visual
inspection to determine exfoliation corrosion susceptibility according to a series of standard photographs.
It should be noted that heating 5xxx alloys with more
than 3% magnesium content for extended periods of
time at or above 150°F leads to an almost continuous
intergranular precipitation of beta-phase, leading to a
condition called sensitization, which makes the alloy
susceptible to intergranular corrosion, exfoliation corrosion, and stress corrosion cracking. Although the special
tempers (either H116 or H321) avoid grain boundary
precipitation of beta-phase in the as-received condition,
they do not preclude eventual sensitization if the product
is held at temperatures at or above 150°F.
For non-marine applications and per ASTM B 209, the
5xxx-H32 temper is available, although the choice between 5xxx-H321 per ASTM B 928 and 5xxx-H32 can be
made depending on the need for corrosion testing.
Solution Heat Treatment and Aging of
Strain Hardenable Aluminum Alloys
The solubility of alloying and trace elements in 1xxx,
3xxx, and 5xxx alloy solid solutions decreases rapidly
with decreasing temperature, which results in most cases
in some degree of supersaturation of these elements at
room temperature upon cooling after hot working or annealing. Although these alloys are strain hardenable but
not age hardenable in the conventional sense, a slight
amount of age hardening may occur in the supersaturated solution due to negligible precipitation of some
age hardenable phases, depending on the composition
of some trace elements such as Si and Cu. No special temper designations are used for such heat treatments.
Strain Hardening Tempers of
Age Hardenable Aluminum Alloys
Special products made of age hardenable aluminum
alloys, normally available in F, O, and T tempers, are also
available to a limited extent in H tempers.2 For example,
extruded 6101 alloy products are available in the H111
temper (annealed and cold worked by a small amount
during straightening or other processing so as not to
qualify as annealed or O temper). Some 2xxx, 6xxx,
and 7xxx alloys in rivet and cold heading wire and rod
are available in H13, H15, and H23 tempers to achieve
high formability but with higher strength relative to the
O temper. The fin stock/cladding alloy 7072 is a special
case of a 7xxx alloy that is not available in T tempers but
only in the O and H tempers.
of this article
by Mike Skillingberg
Editor’s Note: For The
go to The
1. ANSI H35.1/H35.1(M)-2009, Revision of H35.1/
H35.1(M)-2006, American National Standard Alloy and Temper Designation Systems for Aluminum, Secretariat, The Aluminum Association, Inc., Approved April 7, 2009.
2. Aluminum Standards and Data 2009, The Aluminum
Association, Inc., 2009 (www.aluminum.org ordered
through their Bookstore window).
3. Shafiee, P., P. Pollak, and M. Skillingberg, “Temper
Registration Records,” Light Metal Age, April 2003, p. 4042.
4. Hesse, W. (ed.), Key to Aluminium Alloys (AluminiumSchlüssel), 7th Edition, Aluminium-Verlag Marketing &
Kommunikation GmbH, Düsseldorf, Germany, 2006.
5. Hesse, W. (ed.), Key to Aluminium Alloys (AluminiumSchlüssel), 8th Edition, Aluminium-Verlag Marketing &
Kommunikation GmbH, Düsseldorf, Germany, 2008.
6. European Aluminium Association (EAA) Activity Report
7. Aluminium-Taschenbuch (Aluminum Handbook), Aluminium-Verlag Marketing & Kommunikation GmbH,
Düsseldorf, Germany (in German), 1988.
8. Skillingberg, M., “The Aluminum Industry Continues Support for the Marine Market: New Temper Definitions Published,” The Aluminum Association, September
15, 2005 (open letter).
9. ASTM B 928/B 928M-07, Standard Specification for
High Magnesium Aluminum-Alloy Sheet and Plate for Marine
Service and Similar Environments, June 2007.
10. ASTM G 66-99 (Reapproved 2005), Standard Test
Method for Visual Assessment of Exfoliation Corrosion Susceptibility of 5XXX Series Aluminum Alloys (ASSET Test), May
11. ASTM G 67-04, Standard Test Method for Determining
Susceptibility to Intergranular Corrosion of 5XXX Series Aluminum Alloys by Mass Loss after Exposure to Nitric Acid (NAMLT
Test), May 2004.
LIGHT METAL AGE, OCTOBER 2009